# Electronic Supplementary Material (ESI) for RSC Advances.
# This journal is © The Royal Society of Chemistry 2015

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_140307g
_database_code_depnum_ccdc_archive 'CCDC 1055385'
_audit_update_record             
;
2015-03-22 deposited with the CCDC.
2015-05-15 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C20 H28 Mo8 N8 O26'
_chemical_formula_weight         1564.02

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Triclinic
_symmetry_space_group_name_H-M   P-1

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   9.906(4)
_cell_length_b                   10.108(4)
_cell_length_c                   10.995(4)
_cell_angle_alpha                66.978(4)
_cell_angle_beta                 84.193(5)
_cell_angle_gamma                74.144(4)
_cell_volume                     974.7(6)
_cell_formula_units_Z            1
_cell_measurement_temperature    298(2)
_cell_measurement_reflns_used    2418
_cell_measurement_theta_min      2.927
_cell_measurement_theta_max      28.052

_exptl_crystal_description       block
_exptl_crystal_colour            yellow
_exptl_crystal_size_max          0.40
_exptl_crystal_size_mid          0.36
_exptl_crystal_size_min          0.21
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    2.665
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             748
_exptl_absorpt_coefficient_mu    2.591
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.4239
_exptl_absorpt_correction_T_max  0.6122
_exptl_absorpt_process_details   sadabs

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      298(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            4863
_diffrn_reflns_av_R_equivalents  0.0255
_diffrn_reflns_av_sigmaI/netI    0.0505
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_theta_min         2.93
_diffrn_reflns_theta_max         25.02
_reflns_number_total             3351
_reflns_number_gt                2368
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0786P)²+0.1245P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    mixed
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         3351
_refine_ls_number_parameters     280
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0640
_refine_ls_R_factor_gt           0.0419
_refine_ls_wR_factor_ref         0.1392
_refine_ls_wR_factor_gt          0.1172
_refine_ls_goodness_of_fit_ref   1.078
_refine_ls_restrained_S_all      1.078
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.48071(7) 0.57678(7) 0.22374(6) 0.0242(2) Uani 1 1 d . . .
Mo2 Mo 0.20537(7) 0.57945(7) 0.44158(6) 0.0237(2) Uani 1 1 d . . .
Mo3 Mo 0.53303(7) 0.31321(7) 0.50854(6) 0.0206(2) Uani 1 1 d . . .
Mo4 Mo 0.25738(8) 0.30798(8) 0.72986(7) 0.0272(2) Uani 1 1 d . . .
N1 N 0.1413(9) 0.3080(9) 0.3093(9) 0.049(2) Uani 1 1 d . . .
H1 H 0.0662 0.3443 0.3443 0.059 Uiso 1 1 calc R . .
N2 N 0.4878(11) 0.1262(11) 0.1432(10) 0.091(4) Uani 1 1 d . . .
H2A H 0.5491 0.0493 0.1915 0.109 Uiso 1 1 calc R . .
H2B H 0.4994 0.1640 0.0591 0.109 Uiso 1 1 calc R . .
N3 N 0.1580(9) 0.7887(9) 0.7756(7) 0.047(2) Uani 1 1 d . . .
H3 H 0.2324 0.7410 0.7484 0.056 Uiso 1 1 calc R . .
N4 N -0.1912(9) 1.0179(10) 0.9039(9) 0.066(3) Uani 1 1 d . . .
H4A H -0.2473 1.0930 0.8476 0.079 Uiso 1 1 calc R . .
H4B H -0.2090 0.9918 0.9870 0.079 Uiso 1 1 calc R . .
O1 O 0.3939(6) 0.4328(6) 0.3687(5) 0.0251(12) Uani 1 1 d . . .
O2 O 0.3447(5) 0.7003(5) 0.3563(5) 0.0230(12) Uani 1 1 d . . .
O3 O 0.6070(5) 0.5121(5) 0.4089(5) 0.0222(12) Uani 1 1 d . . .
O4 O 0.5923(6) 0.4526(6) 0.1670(5) 0.0360(14) Uani 1 1 d . . .
O5 O 0.3472(7) 0.6655(7) 0.1124(6) 0.0433(16) Uani 1 1 d . . .
O6 O 0.5751(6) 0.7303(6) 0.1728(5) 0.0296(13) Uani 1 1 d . . .
O7 O 0.1780(6) 0.3926(6) 0.5559(5) 0.0300(13) Uani 1 1 d . . .
O8 O 0.1060(6) 0.6913(6) 0.5172(5) 0.0318(14) Uani 1 1 d . . .
O9 O 0.1138(6) 0.6186(6) 0.3047(5) 0.0373(15) Uani 1 1 d . . .
O10 O 0.4299(6) 0.2007(6) 0.6145(5) 0.0301(13) Uani 1 1 d . . .
O11 O 0.6435(6) 0.2015(6) 0.4386(5) 0.0321(14) Uani 1 1 d . . .
O12 O 0.1484(6) 0.4251(7) 0.7957(6) 0.0380(15) Uani 1 1 d . . .
O13 O 0.2145(7) 0.1416(7) 0.8026(6) 0.0423(16) Uani 1 1 d . . .
C1 C 0.1594(10) 0.3692(10) 0.1812(10) 0.045(2) Uani 1 1 d . . .
H1A H 0.0925 0.4529 0.1305 0.054 Uiso 1 1 calc R . .
C2 C 0.2733(11) 0.3126(10) 0.1223(9) 0.051(3) Uani 1 1 d . . .
H2 H 0.2845 0.3568 0.0315 0.061 Uiso 1 1 calc R . .
C3 C 0.3754(11) 0.1863(10) 0.1982(9) 0.046(3) Uani 1 1 d . . .
C4 C 0.3533(11) 0.1278(10) 0.3341(9) 0.044(2) Uani 1 1 d . . .
H4 H 0.4188 0.0455 0.3884 0.053 Uiso 1 1 calc R . .
C5 C 0.2373(12) 0.1902(11) 0.3866(9) 0.047(3) Uani 1 1 d . . .
H5 H 0.2235 0.1513 0.4775 0.056 Uiso 1 1 calc R . .
C6 C 0.0706(11) 0.9053(11) 0.6884(9) 0.046(2) Uani 1 1 d . . .
H6 H 0.0912 0.9327 0.5988 0.055 Uiso 1 1 calc R . .
C7 C -0.0481(11) 0.9856(10) 0.7268(9) 0.047(3) Uani 1 1 d . . .
H7 H -0.1079 1.0663 0.6647 0.056 Uiso 1 1 calc R . .
C8 C -0.0779(10) 0.9431(9) 0.8630(9) 0.037(2) Uani 1 1 d . . .
C9 C 0.0171(10) 0.8193(10) 0.9519(8) 0.040(2) Uani 1 1 d . . .
H9 H 0.0012 0.7888 1.0424 0.048 Uiso 1 1 calc R . .
C10 C 0.1304(10) 0.7459(10) 0.9051(9) 0.043(2) Uani 1 1 d . . .
H10 H 0.1913 0.6630 0.9641 0.052 Uiso 1 1 calc R . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O5 1.695(6) . ?
Mo1 O4 1.703(6) . ?
Mo1 O6 1.899(5) . ?
Mo1 O1 1.998(5) . ?
Mo1 O3 2.273(5) . ?
Mo1 O2 2.368(5) . ?
Mo1 Mo3 3.1970(12) . ?
Mo2 O9 1.691(6) . ?
Mo2 O8 1.703(5) . ?
Mo2 O7 1.891(5) . ?
Mo2 O2 2.010(5) . ?
Mo2 O1 2.332(5) . ?
Mo2 O3 2.345(5) 2_666 ?
Mo3 O11 1.702(5) . ?
Mo3 O10 1.747(5) . ?
Mo3 O1 1.946(5) . ?
Mo3 O2 1.951(5) 2_666 ?
Mo3 O3 2.168(5) . ?
Mo3 O3 2.350(5) 2_666 ?
Mo4 O12 1.704(6) . ?
Mo4 O13 1.708(6) . ?
Mo4 O7 1.915(6) . ?
Mo4 O6 1.932(6) 2_666 ?
Mo4 O10 2.309(6) . ?
Mo4 O3 2.488(5) 2_666 ?
N1 C1 1.314(12) . ?
N1 C5 1.341(13) . ?
N1 H1 0.8600 . ?
N2 C3 1.325(12) . ?
N2 H2A 0.8600 . ?
N2 H2B 0.8600 . ?
N3 C6 1.336(11) . ?
N3 C10 1.339(11) . ?
N3 H3 0.8600 . ?
N4 C8 1.317(11) . ?
N4 H4A 0.8600 . ?
N4 H4B 0.8600 . ?
O2 Mo3 1.951(5) 2_666 ?
O3 Mo2 2.345(5) 2_666 ?
O3 Mo3 2.350(5) 2_666 ?
O3 Mo4 2.488(5) 2_666 ?
O6 Mo4 1.932(6) 2_666 ?
C1 C2 1.345(13) . ?
C1 H1A 0.9300 . ?
C2 C3 1.408(13) . ?
C2 H2 0.9300 . ?
C3 C4 1.394(12) . ?
C4 C5 1.344(14) . ?
C4 H4 0.9300 . ?
C5 H5 0.9300 . ?
C6 C7 1.365(13) . ?
C6 H6 0.9300 . ?
C7 C8 1.411(12) . ?
C7 H7 0.9300 . ?
C8 C9 1.412(12) . ?
C9 C10 1.342(12) . ?
C9 H9 0.9300 . ?
C10 H10 0.9300 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O5 Mo1 O4 105.5(3) . . ?
O5 Mo1 O6 98.4(3) . . ?
O4 Mo1 O6 101.5(3) . . ?
O5 Mo1 O1 101.2(3) . . ?
O4 Mo1 O1 97.7(3) . . ?
O6 Mo1 O1 147.7(2) . . ?
O5 Mo1 O3 158.8(3) . . ?
O4 Mo1 O3 95.7(2) . . ?
O6 Mo1 O3 78.2(2) . . ?
O1 Mo1 O3 74.2(2) . . ?
O5 Mo1 O2 86.8(2) . . ?
O4 Mo1 O2 165.2(2) . . ?
O6 Mo1 O2 84.4(2) . . ?
O1 Mo1 O2 71.35(19) . . ?
O3 Mo1 O2 72.00(18) . . ?
O5 Mo1 Mo3 136.5(2) . . ?
O4 Mo1 Mo3 85.66(19) . . ?
O6 Mo1 Mo3 120.87(16) . . ?
O1 Mo1 Mo3 35.31(15) . . ?
O3 Mo1 Mo3 42.67(12) . . ?
O2 Mo1 Mo3 79.67(12) . . ?
O9 Mo2 O8 105.3(3) . . ?
O9 Mo2 O7 103.1(3) . . ?
O8 Mo2 O7 100.9(2) . . ?
O9 Mo2 O2 98.5(3) . . ?
O8 Mo2 O2 97.8(2) . . ?
O7 Mo2 O2 146.5(2) . . ?
O9 Mo2 O1 89.6(2) . . ?
O8 Mo2 O1 163.3(2) . . ?
O7 Mo2 O1 82.8(2) . . ?
O2 Mo2 O1 71.9(2) . . ?
O9 Mo2 O3 160.2(2) . 2_666 ?
O8 Mo2 O3 93.9(2) . 2_666 ?
O7 Mo2 O3 77.7(2) . 2_666 ?
O2 Mo2 O3 73.45(19) . 2_666 ?
O1 Mo2 O3 70.80(18) . 2_666 ?
O11 Mo3 O10 104.0(3) . . ?
O11 Mo3 O1 101.3(2) . . ?
O10 Mo3 O1 97.4(2) . . ?
O11 Mo3 O2 100.8(3) . 2_666 ?
O10 Mo3 O2 97.1(2) . 2_666 ?
O1 Mo3 O2 149.6(2) . 2_666 ?
O11 Mo3 O3 98.6(2) . . ?
O10 Mo3 O3 157.4(2) . . ?
O1 Mo3 O3 77.7(2) . . ?
O2 Mo3 O3 78.73(19) 2_666 . ?
O11 Mo3 O3 173.7(2) . 2_666 ?
O10 Mo3 O3 82.3(2) . 2_666 ?
O1 Mo3 O3 77.56(19) . 2_666 ?
O2 Mo3 O3 78.15(19) 2_666 2_666 ?
O3 Mo3 O3 75.1(2) . 2_666 ?
O11 Mo3 Mo1 89.32(18) . . ?
O10 Mo3 Mo1 133.76(19) . . ?
O1 Mo3 Mo1 36.38(15) . . ?
O2 Mo3 Mo1 124.01(15) 2_666 . ?
O3 Mo3 Mo1 45.28(13) . . ?
O3 Mo3 Mo1 86.21(12) 2_666 . ?
O12 Mo4 O13 106.3(3) . . ?
O12 Mo4 O7 99.2(3) . . ?
O13 Mo4 O7 104.7(3) . . ?
O12 Mo4 O6 97.6(3) . 2_666 ?
O13 Mo4 O6 101.4(3) . 2_666 ?
O7 Mo4 O6 143.4(2) . 2_666 ?
O12 Mo4 O10 165.2(2) . . ?
O13 Mo4 O10 88.4(2) . . ?
O7 Mo4 O10 77.7(2) . . ?
O6 Mo4 O10 77.9(2) 2_666 . ?
O12 Mo4 O3 95.8(2) . 2_666 ?
O13 Mo4 O3 157.7(2) . 2_666 ?
O7 Mo4 O3 73.8(2) . 2_666 ?
O6 Mo4 O3 72.38(19) 2_666 2_666 ?
O10 Mo4 O3 69.42(17) . 2_666 ?
C1 N1 C5 121.5(8) . . ?
C1 N1 H1 119.3 . . ?
C5 N1 H1 119.3 . . ?
C3 N2 H2A 120.0 . . ?
C3 N2 H2B 120.0 . . ?
H2A N2 H2B 120.0 . . ?
C6 N3 C10 120.3(8) . . ?
C6 N3 H3 119.8 . . ?
C10 N3 H3 119.8 . . ?
C8 N4 H4A 120.0 . . ?
C8 N4 H4B 120.0 . . ?
H4A N4 H4B 120.0 . . ?
Mo3 O1 Mo1 108.3(3) . . ?
Mo3 O1 Mo2 111.0(2) . . ?
Mo1 O1 Mo2 105.2(2) . . ?
Mo3 O2 Mo2 109.6(2) 2_666 . ?
Mo3 O2 Mo1 108.3(2) 2_666 . ?
Mo2 O2 Mo1 103.5(2) . . ?
Mo3 O3 Mo1 92.06(18) . . ?
Mo3 O3 Mo2 91.59(17) . 2_666 ?
Mo1 O3 Mo2 161.7(2) . 2_666 ?
Mo3 O3 Mo3 104.9(2) . 2_666 ?
Mo1 O3 Mo3 98.75(19) . 2_666 ?
Mo2 O3 Mo3 97.58(18) 2_666 2_666 ?
Mo3 O3 Mo4 163.6(3) . 2_666 ?
Mo1 O3 Mo4 86.84(16) . 2_666 ?
Mo2 O3 Mo4 84.63(16) 2_666 2_666 ?
Mo3 O3 Mo4 91.47(17) 2_666 2_666 ?
Mo1 O6 Mo4 117.6(3) . 2_666 ?
Mo2 O7 Mo4 117.6(3) . . ?
Mo3 O10 Mo4 116.8(3) . . ?
N1 C1 C2 120.9(9) . . ?
N1 C1 H1A 119.5 . . ?
C2 C1 H1A 119.5 . . ?
C1 C2 C3 120.0(9) . . ?
C1 C2 H2 120.0 . . ?
C3 C2 H2 120.0 . . ?
N2 C3 C4 121.5(9) . . ?
N2 C3 C2 121.6(9) . . ?
C4 C3 C2 116.9(9) . . ?
C5 C4 C3 120.1(9) . . ?
C5 C4 H4 120.0 . . ?
C3 C4 H4 120.0 . . ?
N1 C5 C4 120.6(9) . . ?
N1 C5 H5 119.7 . . ?
C4 C5 H5 119.7 . . ?
N3 C6 C7 122.0(8) . . ?
N3 C6 H6 119.0 . . ?
C7 C6 H6 119.0 . . ?
C6 C7 C8 118.4(9) . . ?
C6 C7 H7 120.8 . . ?
C8 C7 H7 120.8 . . ?
N4 C8 C7 120.2(9) . . ?
N4 C8 C9 121.9(8) . . ?
C7 C8 C9 117.9(8) . . ?
C10 C9 C8 119.6(8) . . ?
C10 C9 H9 120.2 . . ?
C8 C9 H9 120.2 . . ?
N3 C10 C9 121.8(8) . . ?
N3 C10 H10 119.1 . . ?
C9 C10 H10 119.1 . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O5 Mo1 Mo3 O11 108.5(4) . . . . ?
O4 Mo1 Mo3 O11 0.4(3) . . . . ?
O6 Mo1 Mo3 O11 -100.3(3) . . . . ?
O1 Mo1 Mo3 O11 110.4(3) . . . . ?
O3 Mo1 Mo3 O11 -102.8(3) . . . . ?
O2 Mo1 Mo3 O11 -177.4(2) . . . . ?
O5 Mo1 Mo3 O10 -0.4(4) . . . . ?
O4 Mo1 Mo3 O10 -108.4(3) . . . . ?
O6 Mo1 Mo3 O10 150.8(3) . . . . ?
O1 Mo1 Mo3 O10 1.5(3) . . . . ?
O3 Mo1 Mo3 O10 148.3(3) . . . . ?
O2 Mo1 Mo3 O10 73.7(3) . . . . ?
O5 Mo1 Mo3 O1 -1.9(4) . . . . ?
O4 Mo1 Mo3 O1 -109.9(3) . . . . ?
O6 Mo1 Mo3 O1 149.3(3) . . . . ?
O3 Mo1 Mo3 O1 146.8(3) . . . . ?
O2 Mo1 Mo3 O1 72.2(3) . . . . ?
O5 Mo1 Mo3 O2 -149.0(4) . . . 2_666 ?
O4 Mo1 Mo3 O2 103.0(3) . . . 2_666 ?
O6 Mo1 Mo3 O2 2.3(3) . . . 2_666 ?
O1 Mo1 Mo3 O2 -147.1(3) . . . 2_666 ?
O3 Mo1 Mo3 O2 -0.2(3) . . . 2_666 ?
O2 Mo1 Mo3 O2 -74.8(2) . . . 2_666 ?
O5 Mo1 Mo3 O3 -148.7(4) . . . . ?
O4 Mo1 Mo3 O3 103.3(3) . . . . ?
O6 Mo1 Mo3 O3 2.5(3) . . . . ?
O1 Mo1 Mo3 O3 -146.8(3) . . . . ?
O2 Mo1 Mo3 O3 -74.6(2) . . . . ?
O5 Mo1 Mo3 O3 -76.0(3) . . . 2_666 ?
O4 Mo1 Mo3 O3 176.0(2) . . . 2_666 ?
O6 Mo1 Mo3 O3 75.2(2) . . . 2_666 ?
O1 Mo1 Mo3 O3 -74.1(3) . . . 2_666 ?
O3 Mo1 Mo3 O3 72.7(3) . . . 2_666 ?
O2 Mo1 Mo3 O3 -1.86(18) . . . 2_666 ?
O11 Mo3 O1 Mo1 -73.0(3) . . . . ?
O10 Mo3 O1 Mo1 -178.9(2) . . . . ?
O2 Mo3 O1 Mo1 63.1(5) 2_666 . . . ?
O3 Mo3 O1 Mo1 23.4(2) . . . . ?
O3 Mo3 O1 Mo1 100.7(2) 2_666 . . . ?
O11 Mo3 O1 Mo2 172.1(2) . . . . ?
O10 Mo3 O1 Mo2 66.1(3) . . . . ?
O2 Mo3 O1 Mo2 -51.8(5) 2_666 . . . ?
O3 Mo3 O1 Mo2 -91.5(2) . . . . ?
O3 Mo3 O1 Mo2 -14.3(2) 2_666 . . . ?
Mo1 Mo3 O1 Mo2 -115.0(3) . . . . ?
O5 Mo1 O1 Mo3 178.7(3) . . . . ?
O4 Mo1 O1 Mo3 71.1(3) . . . . ?
O6 Mo1 O1 Mo3 -55.1(5) . . . . ?
O3 Mo1 O1 Mo3 -22.7(2) . . . . ?
O2 Mo1 O1 Mo3 -98.6(3) . . . . ?
O5 Mo1 O1 Mo2 -62.6(3) . . . . ?
O4 Mo1 O1 Mo2 -170.2(3) . . . . ?
O6 Mo1 O1 Mo2 63.6(5) . . . . ?
O3 Mo1 O1 Mo2 96.1(2) . . . . ?
O2 Mo1 O1 Mo2 20.14(18) . . . . ?
Mo3 Mo1 O1 Mo2 118.7(3) . . . . ?
O9 Mo2 O1 Mo3 -167.9(3) . . . . ?
O8 Mo2 O1 Mo3 39.0(9) . . . . ?
O7 Mo2 O1 Mo3 -64.7(3) . . . . ?
O2 Mo2 O1 Mo3 93.1(3) . . . . ?
O3 Mo2 O1 Mo3 14.8(2) 2_666 . . . ?
O9 Mo2 O1 Mo1 75.2(3) . . . . ?
O8 Mo2 O1 Mo1 -77.9(8) . . . . ?
O7 Mo2 O1 Mo1 178.4(3) . . . . ?
O2 Mo2 O1 Mo1 -23.9(2) . . . . ?
O3 Mo2 O1 Mo1 -102.1(2) 2_666 . . . ?
O9 Mo2 O2 Mo3 177.7(3) . . . 2_666 ?
O8 Mo2 O2 Mo3 70.9(3) . . . 2_666 ?
O7 Mo2 O2 Mo3 -52.7(5) . . . 2_666 ?
O1 Mo2 O2 Mo3 -95.6(2) . . . 2_666 ?
O3 Mo2 O2 Mo3 -20.9(2) 2_666 . . 2_666 ?
O9 Mo2 O2 Mo1 -67.0(3) . . . . ?
O8 Mo2 O2 Mo1 -173.8(2) . . . . ?
O7 Mo2 O2 Mo1 62.7(5) . . . . ?
O1 Mo2 O2 Mo1 19.79(18) . . . . ?
O3 Mo2 O2 Mo1 94.5(2) 2_666 . . . ?
O5 Mo1 O2 Mo3 -164.1(3) . . . 2_666 ?
O4 Mo1 O2 Mo3 49.0(10) . . . 2_666 ?
O6 Mo1 O2 Mo3 -65.4(3) . . . 2_666 ?
O1 Mo1 O2 Mo3 92.9(2) . . . 2_666 ?
O3 Mo1 O2 Mo3 14.0(2) . . . 2_666 ?
Mo3 Mo1 O2 Mo3 57.42(18) . . . 2_666 ?
O5 Mo1 O2 Mo2 79.6(3) . . . . ?
O4 Mo1 O2 Mo2 -67.3(10) . . . . ?
O6 Mo1 O2 Mo2 178.3(2) . . . . ?
O1 Mo1 O2 Mo2 -23.4(2) . . . . ?
O3 Mo1 O2 Mo2 -102.3(2) . . . . ?
Mo3 Mo1 O2 Mo2 -58.88(16) . . . . ?
O11 Mo3 O3 Mo1 80.4(2) . . . . ?
O10 Mo3 O3 Mo1 -98.8(6) . . . . ?
O1 Mo3 O3 Mo1 -19.40(19) . . . . ?
O2 Mo3 O3 Mo1 179.8(2) 2_666 . . . ?
O3 Mo3 O3 Mo1 -99.6(2) 2_666 . . . ?
O11 Mo3 O3 Mo2 -81.7(2) . . . 2_666 ?
O10 Mo3 O3 Mo2 99.1(6) . . . 2_666 ?
O1 Mo3 O3 Mo2 178.5(2) . . . 2_666 ?
O2 Mo3 O3 Mo2 17.70(19) 2_666 . . 2_666 ?
O3 Mo3 O3 Mo2 98.3(2) 2_666 . . 2_666 ?
Mo1 Mo3 O3 Mo2 -162.1(3) . . . 2_666 ?
O11 Mo3 O3 Mo3 -180.0(2) . . . 2_666 ?
O10 Mo3 O3 Mo3 0.8(7) . . . 2_666 ?
O1 Mo3 O3 Mo3 80.2(2) . . . 2_666 ?
O2 Mo3 O3 Mo3 -80.6(2) 2_666 . . 2_666 ?
O3 Mo3 O3 Mo3 0.0 2_666 . . 2_666 ?
Mo1 Mo3 O3 Mo3 99.6(2) . . . 2_666 ?
O11 Mo3 O3 Mo4 -5.4(9) . . . 2_666 ?
O10 Mo3 O3 Mo4 175.4(7) . . . 2_666 ?
O1 Mo3 O3 Mo4 -105.2(8) . . . 2_666 ?
O2 Mo3 O3 Mo4 94.0(8) 2_666 . . 2_666 ?
O3 Mo3 O3 Mo4 174.6(10) 2_666 . . 2_666 ?
Mo1 Mo3 O3 Mo4 -85.8(8) . . . 2_666 ?
O5 Mo1 O3 Mo3 99.3(7) . . . . ?
O4 Mo1 O3 Mo3 -77.3(2) . . . . ?
O6 Mo1 O3 Mo3 -177.8(2) . . . . ?
O1 Mo1 O3 Mo3 19.19(19) . . . . ?
O2 Mo1 O3 Mo3 94.3(2) . . . . ?
O5 Mo1 O3 Mo2 -159.3(8) . . . 2_666 ?
O4 Mo1 O3 Mo2 24.1(8) . . . 2_666 ?
O6 Mo1 O3 Mo2 -76.4(8) . . . 2_666 ?
O1 Mo1 O3 Mo2 120.6(8) . . . 2_666 ?
O2 Mo1 O3 Mo2 -164.3(8) . . . 2_666 ?
Mo3 Mo1 O3 Mo2 101.4(8) . . . 2_666 ?
O5 Mo1 O3 Mo3 -6.1(8) . . . 2_666 ?
O4 Mo1 O3 Mo3 177.3(2) . . . 2_666 ?
O6 Mo1 O3 Mo3 76.8(2) . . . 2_666 ?
O1 Mo1 O3 Mo3 -86.2(2) . . . 2_666 ?
O2 Mo1 O3 Mo3 -11.14(17) . . . 2_666 ?
Mo3 Mo1 O3 Mo3 -105.4(2) . . . 2_666 ?
O5 Mo1 O3 Mo4 -97.1(7) . . . 2_666 ?
O4 Mo1 O3 Mo4 86.3(2) . . . 2_666 ?
O6 Mo1 O3 Mo4 -14.2(2) . . . 2_666 ?
O1 Mo1 O3 Mo4 -177.2(2) . . . 2_666 ?
O2 Mo1 O3 Mo4 -102.15(18) . . . 2_666 ?
Mo3 Mo1 O3 Mo4 163.6(2) . . . 2_666 ?
O5 Mo1 O6 Mo4 179.6(3) . . . 2_666 ?
O4 Mo1 O6 Mo4 -72.6(3) . . . 2_666 ?
O1 Mo1 O6 Mo4 52.7(6) . . . 2_666 ?
O3 Mo1 O6 Mo4 20.9(3) . . . 2_666 ?
O2 Mo1 O6 Mo4 93.6(3) . . . 2_666 ?
Mo3 Mo1 O6 Mo4 19.2(4) . . . 2_666 ?
O9 Mo2 O7 Mo4 -177.0(3) . . . . ?
O8 Mo2 O7 Mo4 -68.3(3) . . . . ?
O2 Mo2 O7 Mo4 54.5(5) . . . . ?
O1 Mo2 O7 Mo4 95.2(3) . . . . ?
O3 Mo2 O7 Mo4 23.4(3) 2_666 . . . ?
O12 Mo4 O7 Mo2 71.1(4) . . . . ?
O13 Mo4 O7 Mo2 -179.2(3) . . . . ?
O6 Mo4 O7 Mo2 -45.2(5) 2_666 . . . ?
O10 Mo4 O7 Mo2 -94.2(3) . . . . ?
O3 Mo4 O7 Mo2 -22.4(3) 2_666 . . . ?
O11 Mo3 O10 Mo4 -178.5(3) . . . . ?
O1 Mo3 O10 Mo4 -74.8(3) . . . . ?
O2 Mo3 O10 Mo4 78.4(3) 2_666 . . . ?
O3 Mo3 O10 Mo4 0.7(8) . . . . ?
O3 Mo3 O10 Mo4 1.5(2) 2_666 . . . ?
Mo1 Mo3 O10 Mo4 -75.7(3) . . . . ?
O12 Mo4 O10 Mo3 -3.6(11) . . . . ?
O13 Mo4 O10 Mo3 -179.0(3) . . . . ?
O7 Mo4 O10 Mo3 75.6(3) . . . . ?
O6 Mo4 O10 Mo3 -77.0(3) 2_666 . . . ?
O3 Mo4 O10 Mo3 -1.5(2) 2_666 . . . ?
C5 N1 C1 C2 2.2(15) . . . . ?
N1 C1 C2 C3 -0.3(16) . . . . ?
C1 C2 C3 N2 179.0(11) . . . . ?
C1 C2 C3 C4 -1.4(15) . . . . ?
N2 C3 C4 C5 -179.2(10) . . . . ?
C2 C3 C4 C5 1.2(15) . . . . ?
C1 N1 C5 C4 -2.4(15) . . . . ?
C3 C4 C5 N1 0.6(15) . . . . ?
C10 N3 C6 C7 0.7(15) . . . . ?
N3 C6 C7 C8 0.2(16) . . . . ?
C6 C7 C8 N4 179.8(10) . . . . ?
C6 C7 C8 C9 -0.2(14) . . . . ?
N4 C8 C9 C10 179.4(10) . . . . ?
C7 C8 C9 C10 -0.6(14) . . . . ?
C6 N3 C10 C9 -1.5(15) . . . . ?
C8 C9 C10 N3 1.5(15) . . . . ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
N1 H1 O8 0.86 2.18 2.949(9) 149.2 2_566
N2 H2A O10 0.86 2.56 3.281(10) 141.7 2_656
N2 H2A O13 0.86 2.58 3.333(11) 146.3 2_656
N2 H2B O6 0.86 2.45 3.250(12) 154.9 2_665
N3 H3 O4 0.86 2.18 2.878(10) 138.0 2_666
N3 H3 O11 0.86 2.24 2.900(9) 133.4 2_666
N4 H4A O2 0.86 2.45 3.279(10) 162.5 2_576
N4 H4A O5 0.86 2.56 3.092(11) 120.8 2_576

_diffrn_measured_fraction_theta_max 0.976
_diffrn_reflns_theta_full        25.02
_diffrn_measured_fraction_theta_full 0.976
_refine_diff_density_max         1.493
_refine_diff_density_min         -1.199
_refine_diff_density_rms         0.223
